Crystal growth and luminescence properties of In6W012 T. Gaewdang, J.P. Chaminade,
A. Garcia, C. Fouassier,
Laboratoire de Chimie du Solide du CNRS, Universitk Bordeaux I, 351 Cours de la Liberation, 33405 Talence Cedex, France
and B. Jacquier Laboratoire de Physics-Chimie des Mat&iaux Luminescents, UniversitCLyon I, 43 blvd du I1 Novembre 1918, 69622 Villeurbanne Cedex, France
Received 6 August 1993; accepted 19 August 1993
Single crystals of indium tungstate IQWO,~ have been grown by chemical vapor deposition using TeC& as a transport agent. Isometric as well as octahedral-shaped transparent crystals are obtained with a size attaining 2 mm. The luminescence of both single crystals and powder samples has been investigated. On the basis of a comparison with Y6W01s, the green emission is ascribed to charge transfer transitions within isolated octahedral tungstate groups.
2. Experimental procedure
New attention has been recently paid to transparent crystals containing a large amount of the ’ r51n isotope of indium for detection of low-energy solar neutrinos according to Raghavan’s nuclear reaction [ l-41. A first investigation has been devoted to the growth of InBOa crystals doped with trivalent terbium [ 51. Good quality and large dimensions of transparent crystals led to high luminescent output, but with a long fluorescence decay unsuitable for such detection applications. Recently we have observed an intrinsic luminescence in a double oxide containing In3+ of formula In2Ti05 [ 61. In order to improve understanding of such a phenomenon other indium matrix oxides are to be considered. In this paper we report the crystal growth by chemical vapor transport and the luminescence properties of In6W0,,.
2.1. Sample preparation
2.1.1. Powder formation
Powder samples were prepared by usual solid-state reaction using 99.999% Inz03 from Cerac and analytical grade W03 from Prolabo. Stoichiometric proportions of the starting compounds were ground and fired in a platinum crucible for 2 days at 1050°C in air. After new grinding they were tired again under the same conditions in order to eliminate the last traces of In2 ( W04) 3. Te white powder obtained was checked by X-ray powder diffraction with a Philips diffractometer using Cu Ku radiation. 2.1.2. Crystal growth Crystals were grown by chemical vapor transport in silica ampoules with an internal diameter of about 13 mm and a total length of 110 mm. Approximately 1 g of dried In6W0i2 was introduced into the ampoule together with a calculated amount of TeCL, (99.9% purity Aldrich) in a dry box. This quantity of TeCL, present (5 mg/cm3) corresponds to a total pressure in the ampoule during the transport process
0 1993 Elsevier Science Publishers B.V. All rights reserved.
Volume 18, number 1,2
and before reaction of about 4 atm at 1000°C [ 7 1. It was evacuated, sealed and then heated in a horizontal tubular furnace with two independent heating zones. Before the beginning of the transport process, the growth zone was cleaned “in situ” by back-transport for 24 h. The temperature gradient was then reversed. Once the appropriate temperature established, transport of In6W0i2 began according to an endothermal reaction. The duration of the process for the transport of the whole charge was about 10 days (table 1). After slow cooling to room temperature the ampoule was opened. The crystals were removed from the ampoule walls and cleaned in diluted hydrochloric acid in order to dissolve any condensed chloride or TeOZ, and finally rinsed with distilled water and pure ethanol. 2.2. Luminescence studies Optical measurements were performed as previously described [ 6 3. The diffuse reflectance spectrum of powder was recorded at room temperature on a Cary 2415 spe~trophotometer. The luminescence measurements were carried out from liquid helium temperature up to room temperature on both single crystals and powder samples. The device used consisted essentially of a Jobin-Yvon spectrofluorimeter equipped with an SMC Air Liquide liquid-helium flow cryostat. Decay measurements were performed using a frequency-doubled Quantel model 48 1 YAG:Nd3+ laser which was followed by a three-stage amplifier dye laser (puise width 15 ns, line width 0.1 cm-’ ) to provide a source in visible range (Rhodamine 640)) then the second harmonic of the dye radiation was used to obtain a UV beam at a wavelength of 325
nm. The fluorescence signal was detected by a photocounting system with a multich~nel analyzer (Standford SR 430).
3. Results and discussion 3.1. Crystal growth Various growth conditions have been tested in this investigation and are briefly summarized in table 1. Transport of InsWOlz by TeCI, at lower temperature (run no. 1) favors many colorless transparent octahedral-shaped crystals, whereas at higher temperature (run no. 2) two types of crystals have been found: octahedral-shaped and large blue color isometric crystals up to 2 mm in size (fig. 1). This blue color could be attributed either to nonstoichiometry or to contamination by impurities. Annealing under oxygen at 1000’ C for 24 h leads to transparent crystals in agreement with the oxygen deficiency hypothesis. The lattice parameters obtained for crushed crystals with internal standard agree very well with those reported by Michel and Kahn [S]: aH=9.469(2), c,=8.929(2) ii and a,=9.472(2), c,=8.939(2) A respectively. The crystal symmetry is rhombohedral, with space group R3 (Y6UOi2 type) and Z= 1. The structure
Table 1 Experimental conditions for In,W0,2 growth Run no.
Transport temperature (“C) T,
Duration of growth (days)
Crystal dimension (in size) (mm)
Fig. 1. As-grown crystais of In,WO12 with octahedral (right-hand side) and isometric shape (left-hand side) ( 1 division= 1mm).
Volume 18, number 1,2
determined by previous authors appears as being an anion-deficient fluorite-type with a large supercell. The cationic sublattice ( 1 W and 6 In) is almost facecentered cubic, the oxygen atoms occupy 12 of the 14 formed tetrahedral sites, the two last ones being empty. The lattice contains actually two types of coordination polyhedra: - the W atoms are six-coordinated (with all W-O distances equal to 1.93 8, [ 8 ] ) and form isolated octahedra ( W06)6--, - In is su~ounded by seven 0 atoms, six of them being at a distance between 2.12 and 2.28 A and the last one at 2.77 A. 3.2. Luminescence The diffuse reflectance spectrum of In6W012 powder exhibits at room temperature an optical absorption edge at about 330 nm (fig. 2). By excitation into this absorption band the compound shows a green emission below 1.50 K. At 4.2 K a broad emission band shows a maximum around 500 nm. Because of the large width of this band the emission maximum is not easy to determine accurately. The corresponding excitation band shows a maximum at about 325 nm. This can be considered as being in good agreement with the results of the diffuse reflectance spectrum if the temperature dependence is considered. At 4.2 K the emission intensity is rather high and it stays roughly constant up to about 20 K. From that temperature, thermal quenching appears.
At 60 K the total intensity has dropped to about 50°h of the liquid helium value. The decay time of this luminescence is rather short. At 4.2 K the decay curve consists of an overlapping of fast and slow components characterized by decay times of 10 and 20 ps respectively (fig. 3). At increasing temperature the fluorescence decay becomes single exponential and exhibits a shorter lifetime ( 10 ps at 20 K for example ) . The single crystal emission spectrum is similar to that of the powder, but the excitation maximum appears at 335 nm instead of 325 nm (fig. 2). The difference between the positions of the excitation maximum for powder and crystals results from a wellknown saturation phenomenon: in strongly absorbing crystals excitation into the absorption maximum is not completely effective, as the excitation beam cannot enter fully the crystals. Radiationless losses occur at the crystal surface [ 9 1. In our previous investigation of IntTiOS, the comparison between titanate and indate compounds led us to propose an inte~retation of the luminescence
Fig. 2. Diffuse reflectance spectrum (dashed line) at room temperature, excitation (a) and emission (b) spectra at 4.2 K of In6WO12.For (a) the sofid line corresponds to a powder sample, the dot-dash line to single crystals. The emission spectra of single crystals and powder samples are similar.
Fig. 3. Luminescent decay of In6WO12at 500 nm, i.e. the emission maximum at 4.2 K.
spectrum in terms of a charge transfer from 02- to In3+ occurring in (In,O,)?ribbons of the lattice the obtained luminescent data . For In,WOi,, differ from those of In2TiOs and In203 [6,10]. Blasse et al. [ 1 l-l 41 have investigated the luminescence of various tungstate compounds and particularly of Y6W0,2, but the exact excitation and emission maximum values for the latter were not reported. It was worthwhile, therefore, to reinvestigate the luminescence properties of Y6WOi2, which belongs to the same structural type [ 151, in order to compare them with those of In,WOi,. The luminescence of Y6WOi2 is quite similar to that of In6W0,2 (i.e. band shape, spectral region of the excitation and emission spectra, luminescence decay curves). However, small differences can be observed (see table 2): higher energy of the first absorption band (or excitation maximum), higher thermal quenching temperature, higher intensity and larger decay constants for Y6WOi2 compared to those of In6W0i2. The luminescence of highly charged ions with do configuration as W6+ is well known and has been studied for many years [ 16,171. The optical transitions involved can be attributed to ligand ( 02- ) to metal ( W6+ ) charge transfers. The influence of the energy value of the first absorption band on the efficiency of the luminescence is dramatic. A higher energy position of the first absorption band yields higher thermal quenching temperature of luminescence as already observed experimentally for various closed-shell transition metal ions [ 11,18-23 1. It was argued that this relation can Table 2 Some data for the luminescence
optical absorption edge (nm) at 300 K excitation maximum (nm) emission maximum (nm) Stokes shift value (cm-‘) E,/Z C, decay times, T, for the fast and slow component of the decay (us)
be qualitatively explained by considering a simple configuration coordinate diagram in which the shape of the curve for the equilibrium distance does not depend significantly on the crystal structure [ 11,12,2 1,241. Our experimental data are well in line with those reported previously [ 11,121. The activation energy of the thermal luminescence quenching increases if the position of the emitting level shifts to higher energies [ 111. This activation energy (AE) can be derived from the experimental temperature curve according to the relation: I=&,/ [ 1 +A exp( - AE/kT)
where I is the intensity at a temperature T and I,, the intensity at a sufficiently low temperature (let us say 4.2 K), A is a constant. The activation energy for Y6WOL2 and InsWOi2 is respectively 60 meV (480 cm-‘) and 40 meV (320 cm-‘). The Stokes shift of In6WOi2 is smaller than that of Y6WOi2. In terms of single configurational coordinate diagram it should usually lead to higher quenching temperature, but it is not the case. The position of the lowest absorption band for In6WOi2 is situated at lower energies, however, when compared to that of Y6WOi2. The benefit of a higher energy position for the first absorption then clearly outweighs that of a smaller Stokes shift of the emission. The slow component of the decay at low temperature can be ascribed to the intrinsic luminescence [ 251. For both tungstates the decay time shows a strong variation below 20 K: For Y,WOr2 the decay time drops from 105 us at
at 4.2 K
335 500 9850 4000
- at 4.2 K -at20K T,,z d’(K)
330 325 500 10770 4000
310 305 490 12380 4500
10,20 10 60
29, 105 34 100
a) crystal. b, Powder. ‘) E1i2: emission band width at half height. d, Temperature for which the 4.2 K emission intensity has dropped to 50%.
Volume 18, number 1,2
4.2 K to 34 us at 20 K but decreases slowly after. This behavior clearly characterizes a thermal equilibrium between two close-energy levels with smaller radiative probability for the lowest one. It has already been observed for various closed-shell transition element complexes [ 17,25 1. The temperature dependence was fitted with the parameters: - energy separation of the excited states: E= 9 cm-‘, - radiative probabilities PZl= 5700 s-l ( r2i = 175 us) and P,,=8000 s-l (r3,=12 us). The decay value (T) for the level with the highest radiative probability is comparable to that observed for other undistorted tungstate groups [ 26 1. The shorter luminescence decay of In6W0r2 may be due to nonradiative transitions, resulting from the low position of the emitting state. The proximity of the indium states, which are involved in the luminescence of In2TiOs [ 61, with 02- + W6+ charge transfer states may also affect both radiative and nonradiative properties of In6Woi2.
4. Conclusion Single Cry&d growth of In6WOi2 by chemical vapor transport using TeC& as a transport agent has been performed. Luminescence properties of these single crystals are in agreement with those of powder sample. Comparison of the luminescence of isostructural In6W& and Y6WOi2 leads to the conclusion that the optical transitions responsible for the luminescence of the indium tungstate are of chargetransfer type within isolated octahedral tungstate groups. As a consequence of the lower position of the first absorption band, thermal quenching is more pronounced for In6Woi2 than for Y6W012. A comparison of the luminescence lifetime, which decreases from In6Woi2 to YdW0i2, seems to show that indium orbitals affect the transition probabilities of the charge transfer process. &WC12 appears as a possible candidate for use as a scintillator for detection of neutrinos. As a consequence the growth procedure has to be improved to give rise to larger crystals.
The authors thank Mr. 0. Viraphong for his kind assistance during the crystal growth experiments.
References [ 1 ] L. Gonzalez-Mestres and D. Perret-Gallix, Ann. Phys. 3 (1988) 181. [ 21 L. Gonzalez-Mestres and D. Perret-Gallix, in: Neutrinos ‘88, Boston, 1988 (World Scientific, Singapore, 1989).  L. Gonzalez-Mestres, Nucl. Phys. B (Proc. Suppl.) A 28 ( 1992) 478. [ 41 M. Avenier, G. Bagieu, R. Brissot, J.F. Cavaignac, J. Collot, D.H. Koang, D. Lebrun, F. Minot and A. Stutz, Nucl. Phys. B (Proc. Suppl.) A 28 (1992) 496. [ 5] J.P. Chaminade, A. Garcia, M. Pouchard, C. Fouassier, B. Jacquier, D. Perret-Gallix and L. Gonzalez-Mestres, J. Crystal Growth 99 (1990) 799. [ 61 T. Gaewdang, J.P. Chaminade, P. Gravereau, A. Garcia, C. Fouassier, P. Hagenmuller and R. Mahiou, Mater. Res. Sot. Bull., in press. [ 71 W. Piekarczyk, P. Peshev, A. Toshev and A. Pajaczkowska, Mater. Res. Sot. Bull. 13 (1978) 587. [S] D. Michel and A. Kahn, Acta Ctyst. B 28 (1982) 1437. [ 91 Z.B. Mazuak, G. Blame and J. Liebertz, J. Solid State Chem. 68 (1987) 181. [lo] H. Yamamoto and K. Urabe, J. Electrochem. Sot. 129 (1982) 2069. [ 111 G. Blasse and A. Bril, Z. Physik. Chem. N.F. 57 (1968) 187. [ 121 G. Blasse and A.Bril, J. Electrochem. Sot. 115 (1968) 1067. G.Blasse,Chem.Phys.Letters41 (1976) 210. [ 141 G. Blasse, J. Electrochem. Sot. 124 (1977) 1280. [ 1510. Beauty, M. Faucher and P. Caro, Mater. Res. Sot. Bull. 13 (1978) 175. [ 161 F.A. Krtiger, Some aspects of the luminescence of solids (Elsevier, Amsterdam, 1948). [ 17 ] G. Blasse, Structure Bonding 42 ( 1980) 1. [ 181 G. Blasse, J. Chem. Phys. 5 1 ( 1969) 3529. [ 201 G. Blasse, G.J. Dirksen, M.F. Hazenkamp, A. Verbaere and S. Oyetola, Eur. J. Solid State Inorg. Chem. 26 ( 1989) 497.  M. Wiegel and G. Blasse, J. Solid State Chem. 99 (1992) 388. [ 221 A.M. Srivastava and J.F. Ackerman, Chem. Mater. 4 (1992) 1011.  A.M. Srivastava and J.F. Ackerman, J. Solid State Chem. 98 (1992) 144. [ 241 G. Blasse, Progr. Solid State Chem. 18 ( 1988) 79.  G. Blasse and G. Bokkers, J. Solid State Chem. 49 ( 1983) 126.
Report "Crystal growth and luminescence properties of In6WO12"